{'fraction_non_alphanumeric': 0.026757934038581208, 'fraction_numerical': 0.01431238332296204, 'mean_word_length': 4.8901098901098905, 'pattern_counts': {'":': 0, '<': 0, '<?xml version=': 0, '>': 0, 'https://': 0, 'lorem ipsum': 0, 'www.': 0, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 0, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
Evaluation of shear bond strength between zirconia core and ceramic veneers fabricated by pressing and layering techniques: In vitro study

Statement of Problem: Although ceramic veneered on to zirconia core have been in use for quite some time, information regarding the comparative evaluation of the Shear bond strength of Pressable & Layered ceramic veneered on to zirconia core is limited. Purpose of study: To evaluate the shear bond strength of zirconia core and ceramic veneer fabricated by two different techniques, Layering (Noritake CZR) and Pressing (Noritake, CZR Press). Materials and Method: 20 samples of zirconia blocks were fabricated and the samples were divided into group A & B. Group A - Ceramic Veneered over zirconia core by pressing using Noritake CZR Press. Group B - Ceramic Veneered over zirconia core by layering using Noritake CZR. The veneered specimens were mounted on to the center of a PVC tube using self-cure acrylic resin leaving 3 mm of the veneered surface exposed as cantilever. Using a Universal testing machine the blocks were loaded up to failure. Result: The results were tabulated by using independent samples t-test. The mean shear bond strength for Pressed specimens was 12.458 ± 1.63(S.D) MPa and for layered specimens was 8.458 ± 0.845(S.D) MPa. Conclusion: Pressed specimens performed significantly better than the layered specimen with a P value 0.001. Clinicians and dental laboratory technicians should consider the use of pressed ceramics as an alternative to traditional layering procedures to reduce the chances of chipping or de-lamination of ceramics